Tampere University of Technology
Accelerated deactivation studies of the natural-gas oxidation
catalyst-Verifying the roleof sulfur and elevated temperature in
CitationHonkanen, M., Krkkinen, M., Kolli, T., Heikkinen, O.,
Viitanen, V., Zeng, L., ... Vippola, M. (2016).
Accelerateddeactivation studies of the natural-gas oxidation
catalyst-Verifying the role of sulfur and elevated temperature
incatalyst aging. Applied Catalysis B-Environmental, 439-448. DOI:
VersionPeer reviewed version (post-print)
Link to publicationTUTCRIS Portal
Published inApplied Catalysis B-Environmental
Copyright 2015. This manuscript version is made available under
the CC-BY-NC-ND 4.0
Take down policyIf you believe that this document breaches
copyright, please contact [email protected], and we will remove access
tothe work immediately and investigate your claim.
Accelerated Deactivation Studies of the Natural-Gas Oxidation
Catalyst - Verifying the Role
of Sulfur and Elevated Temperature in Catalyst Aging
Mari Honkanen(a),(*), Marja Krkkinen(b), Tanja Kolli(b), Olli
Heikkinen(c), Ville Viitanen(c), Lunjie
Zeng(d), Hua Jiang(c), Kauko Kallinen(e), Mika Huuhtanen(b),
Riitta L. Keiski(b), Jouko Lahtinen(c),
Eva Olsson(d), Minnamari Vippola(a)
(a) Department of Materials Science, Tampere University of
Technology, P.O. Box 589, 33101
Tampere, Finland(b) Environmental and Chemical Engineering,
Faculty of Technology, University of Oulu,
P.O. Box 4300, 90014 Oulu, Finland(c) Department of Applied
Physics, Aalto University, P.O. Box 14100, 00076 Aalto, Finland(d)
Department of Applied Physics, Chalmers University of Technology,
Sweden(e)Dinex Ecocat Oy, Typpitie 1, 90620 Oulu, Finland
(*) Corresponding author, e-mail: [email protected],
Co-authors e-mails: Marja Krkkinen,
[email protected] Kolli, [email protected]
Heikkinen, [email protected] Viitanen,
[email protected] Zeng, [email protected] Jiang,
[email protected] Kallinen, [email protected] Huuhtanen,
[email protected] L. Keiski, [email protected]
Lahtinen, [email protected] Olsson,
[email protected] Vippola,
In thermal aging, grown particles with Pt/Pd core and PdO shell
Al2(SO4)3 formed near small PtPd particles during
With grown particles, Pt/Pd core + PdO shell, Al2(SO4)3 formed
randomly in catalyst
Combined morphological changes and Al2(SO4)3 formation
Accelerated deactivation, caused by thermal aging (TA) and/or
sulfur+water poisoning (SW), of the
PtPd/g-Al2O3 natural-gas oxidation catalyst was studied. Thermal
aging and poisoning treatments
were performed separately and with varied combinations and
comprehensive characterization of the
catalyst was carried out after each step. The fresh catalyst has
small, oxidized PtPd particles (
Natural gas (NG) is a potential sustainable energy source for
vehicles and engines as its
environmental impacts are smaller than those of e.g. crude
oil-based fuels. For example exhaust
emissions of the natural gas vehicles (NGVs) are much lower than
those in the diesel vehicles.
However, exhaust gases of NGVs contain unburned methane and
carbon monoxide, a potential
greenhouse gases, and thus catalytic oxidation converters are
needed [1,2]. Supported palladium
catalysts are widely known to be active for methane combustion
and it is agreed that PdO is the
active phase while metallic palladium is much less active. PdPdO
transformation is reversible
and according to Farrauto et al. , decomposition temperature
of PdO to Pd in the PdO/Al2O3
catalyst is ~800C and reformation temperature of Pd to PdO
during cooling is ~600C. Hysteresis
in the reformation is due to strongly bound oxygen on the Pd
surface inhibiting bulk oxidation .
Many other factors, such as gas phase composition and pressure,
type of support, additives and
contaminants, and pretreatment conditions, have also effects on
the PdPdO transformation . In
addition, several studies have reported that the activity and
stability of Pd catalysts in methane
combustion can be improved by adding Pt into the catalyst to
decelerate sintering of Pd and PdO,
Deactivation of the catalyst, caused by poisoning and thermal
aging, is a problem also in the natural
gas applications. Poisoning is due to adsorption of impurities,
e.g. S, P, Zn, Ca, and Mg, present in
the exhaust gases, on the catalytic active sites. Poisons can
also react with the active sites followed
by formation of non-active compounds . Sulfur is known to be
one of the most important
components for deactivation of the Pd catalysts for methane
oxidation  and only a small amount
of SO2 significantly decreases catalyst activity by blocking the
active noble metal sites by sulfur
compounds . It is known that sulfur in the NGV exhaust gas
originates from odorants and
lubricating oils and from gas itself. Under the typical
natural-gas engine conditions, with large
excess of air and with an oxidation catalyst, sulfur will be
oxidized to SO2 and SO3. Above 300C, a
catalyst has enough activity for the oxidation of SO2 to SO3
. Metallic Pt on the PtPd catalysts is
found to be active to adsorb sulfur compounds. Therefore, the
presence of metallic Pt prevents
adsorption of sulfur on the Pd surface sites which are then
available for methane oxidation .
Also the catalyst washcoat affects sulfur poisoning. For example
Pd/Al2O3 catalysts deactivate less
than Pd/SiO2 catalysts due to adsorption of SOx also on the
Al2O3 washcoat material .
According to Mowery et al. , when SO2 and water exist, the
sulfation of the PdO/Al2O3 catalyst
happens by oxidation of SO2 to SO3 on PdO and further SO3 over
PdO can form PdSO4 or can
migrate to Al2O3 forming Al2(SO4)3. The sulfation is reversible
and SOx from the catalyst surface
easily desorbs already below 400C and more stable washcoat
sulfates decompose above 700C
. SO2 can affect also the acidity of the Al2O3 support.
Konsolakis et al.  noticed that the
fresh Pd/g-Al2O3 catalyst has only Lewis acid sites but SO2
treatment increases significantly
Brnsted acid sites on the g-Al2O3 support. According to Wischert
et al. , the reactivity of g-
Al2O3 towards methane is due to the highly reactive Lewis
acid-base pairs (Al,O) enabling low-
energy pathways for the dissociation of C-H bond in methane.
Thermal deactivation of a catalyst is reported to be caused by:
a) loss of active surface area due to
crystallite growth of the noble metal particles and due to pore
collapse on crystallites of the active
phase, b) loss of support area due to collapse of the washcoat
and/or c) chemical transformations of
active catalytic phases to non-active phases. In general,
sintering occurs at elevated temperatures
(>500C) and is accelerated by water vapor ; the driving
force for sintering is to minimize
surface energy and it is reduced with the transport, growth, and
coalescence of the particles .
Two mechanisms for sintering of catalyst nanoparticles have been
proposed: particle migration
followed by coalescence (PMC) and Ostwald ripening (OR). In the
particle migration, sintering
occurs by migration of the whole crystallites along the support
surface and coalescence of the
crystallites forms larger particles. OR is migration of single
metal atoms or molecular species from
small particles to large ones; larger particles grow at the
expense of smaller particles [10,1821].
Hansen et al.  studied the mechanism of the catalyst
nanoparticle sintering mainly by in situ
transmission electron microscopy. They noticed that the early
stage of the sintering is dominated by
OR and surface area increases rapidly caused by the
disappearance of the smallest particles. In the
further stage, grown particles coalesce when they are close to
each other. Sintering becomes slower
when particles grow and the distance between them increases
. Many factors e.g. temperature,
atmosphere, metal type, support, and impurities affect the rate
of noble metal sintering. The
sintering rate increases exponentially with elevated temperature
and metals sinter faster in oxygen
than in hydrogen atmosphere . Generally, sintering of the
noble metal clusters is accelerated by
the presence of gases; Parkinson et al.  reported that
existence of carbon monoxide induced
coalescence of Pd atoms in the Pd/Fe3O4 system and that formed
Pd-carbonyl species were
responsible for increased Pd mobility. Water vapor has also been
found to accelerate sintering. In
reducing atmosphere, the stability of the metal crystallites
typically decreases with decreasing noble
metal melting temperature. In oxidizing atmosphere, stability
depends on the volatility of metal
oxides and on the noble metal-support interactions . In
addition, the position of the noble metal
particles affects the rate of sintering; a valley position is
much more stable than an on-top position
. Pores in the support hinder the mobility of the metal
crystallites; especially if pore diameters
are about same size as the crystallites . Impurities affect
the sintering rate, for example sulfur
increases mobility of the metal atoms [18,23,24] while for
example calcium is found to decrease it
In the case of the catalysts with an alumina washcoat, phase
transformations of the support may
occur; g-alumina with high specific surface area can change to
d-alumina and finally via q-alumina
to stable a-alumina . Phase transformation results in
sintering or grain growth followed by a
decrease in the surface area . According to Wischert et al.
, the phase transformation of g-
Al2O3 to q-Al2O3 causes the reconstruction of the surface
resulting in decrease of highly reactive
sites for methane.
In the real vehicle aging conditions, deactivation process is a
complex phenomenon and e.g. both
thermal aging and poisoning exist. In our earlier study ,
the natural-gas heavy-duty-vehicle-
aged (160000 km) PtPd/g-Al2O3-based catalyst was studied.
Significant morphological changes and
chemical poisoning were detected compared to the fresh catalyst
and this has led to drastic
deactivation in methane conversion. It was difficult to conclude
which changes were caused by
thermal aging and which by chemical poisoning. Thus, detailed
studying of deactivation phenomena
in the vehicle-aged catalysts was found very challenging. Sulfur
poisoning of the oxidation catalysts
is widely studied, e.g. [10,11,1315,18]. In this study, sulfur
poisoning and thermal aging were
studied separately and with varied combinations enabling
detailed analysis of the role of sulfur in
the catalyst and effects of thermal aging before or after sulfur
poisoning. This kind of in-depth
knowledge gained is crucial in the development of efficient
exhaust emission reduction systems for
2.1 Catalyst material
The studied material was a PtPd (1:4 wt-%) catalyst supported on
g-alumina washcoat on the
metallic monolith. The studied catalyst was manufactured and
designed by Dinex Ecocat Oy for
lean-burn natural gas applications. Total metal loading in the
catalyst was 8.8 g/dm3 and the catalyst
was calcined at 550C for 4 hours. The catalyst was studied as
fresh and after various chemical and
thermal laboratory-scale accelerated deactivation
2.2 Laboratory-scale accelerated deactivation treatments
Laboratory-scale sulfur + water treatment (SW) and thermal aging
(TA) treatments were carried out
to find out detailed knowledge about deactivation phenomena of
the PtPd/g-Al2O3 oxidation catalyst
for natural-gas applications. SW-treatment was performed in the
following conditions: 100 ppm
SO2, 10 vol-% H2O, 10 vol-% air, balanced with N2. The quartz
tube reactor was heated from room
temperature to 400C in a nitrogen and air flow with the heating
rate of 10C/min. After 5 hours of
the SW-treatment, the reactor was cooled down to the room
temperature in nitrogen and air flow.
The gas hourly space velocity (GHSV) was 20 000 h-1during the
treatment. Thermal aging was
carried out in the tube reactor under synthetic air (80% N2 +
20% O2) at 1000C for 5 hours. The
used temperature was above the normal operation temperature of
the catalysts but it was chosen to
mimic an accelerated thermal aging and thus the long-term
behavior of the catalyst. Temperature
for the TA-treatment was chosen based on our tentative study
about laboratory-scale thermal aging
treatments for natural gas oxidation catalyst (various
temperatures between 400C and 1100C);
with this thermal aging temperature, the catalyst structure
changes similar to a vehicle-aged catalyst
were achieved . The catalyst samples were set into the
tubular ceramic furnace when the
treatment temperature was reached, then the gas flow was
switched on. After the treatment period
the gas flow was switched off and the catalyst samples were
removed from the furnace and let to
cool down to room temperature. TA- and SW-treatments were
performed separately and with varied
combinations (Table 1). Detailed characterization of the
catalyst was carried out after each step.
Table 1. Laboratory-scale treatments and corresponding
markings.Marking TreatmentFresh As-received from Dinex Ecocat OySW
Sulfur + water poisoning (100 ppm SO2 + 10 vol-% H2O + 10 vol-% air
+ N2 (bal.), 400C/5h)TA Thermal aging at 1000C/5h (80 vol-% N2 + 20
vol-% O2)TA+SW Thermal aging followed by sulfur + water
poisoningSW+TA Sulfur + water poisoning followed by thermal aging
The structure of the fresh and treated catalysts was studied by
scanning electron microscopy (SEM),
transmission electron microscopy (TEM), and X-ray diffractometry
(XRD). A field-emission SEM
(FESEM, Zeiss ULTRAplus) is equipped with an energy dispersive
spectrometer (EDS, INCAx-act
silicon-drift detector (SDD), Oxford Instruments).
Cross-sectional FESEM samples were prepared
with a conventional metallographic sample preparation technique
by molding the catalyst samples
into resin followed by grinding and polishing and carbon coating
to avoid sample charging during
the FESEM studies. All the presented cross-sectional FESEM
images were taken with an angular
selective backscatter (AsB) detector to maximize Z-contrast.
Three different TEMs were used to
characterize the samples. A TEM (Jeol JEM-2010) equipped with an
EDS (Noran Vantage Si(Li)
detector, Thermo Scientific) was used for imaging and elemental
analysis. A high resolution TEM
(HRTEM, Jeol 2200FS) with two aberration correctors (CEOS GmbH)
equipped with EDS (Jeol
Si(Li) detector) was used for high resolution imaging and
elemental analysis. A high resolution
TEM/scanning TEM (STEM, FEI Titan 80-300) with a probe Cs
corrector, a Gatan Imaging Filter
(GIF, Tridium), and an EDS (INCAx-sight Si(Li) detector) was
used for high resolution imaging,
electron energy loss spectroscopy (EELS), and elemental
analysis. Annular dark field (ADF) STEM
images were acquired using a 17.5 mrad beam convergence angle
and ~54-270 mrad detector
collection angle. The collection angle for EELS is ~24 mrad.
Cross-sectional TEM samples from
the fresh catalyst and from the TA+SW-treated catalyst were
prepared as follows. Small pieces of
the catalyst monolith were attached the washcoats face-to-face
to a titanium grid by carbon glue.
The grid was pre-thinned by hand to the thickness of ~70 m and
then with a dimple grinder
(Model 565, Gatan Inc.) to the thickness of ~20 m. The final
thinning for electron transparency
was made with a precision ion polishing system (PIPS, Model 691,
Gatan Inc.). Powdered TEM
samples from all studied catalysts were prepared by crushing the
scraped catalyst powder between
two laboratory glass slides and dispersing the crushed powder
with ethanol onto a copper grid with
a holey carbon film. Scraped catalyst powders were used also for
XRD studies (Empyrean with the
PIXcel3D detector, PANanalytical, using Cu Ka radiation).
Crystallite sizes were determined from
the XRD patterns with the aid of the HighScore plus software
based on the Scherrer equation (shape
factor 0.9) and phases were identified by using the database
(PDF-4+ 2014 ) from International
Centre for Diffraction Data (ICDD).
The chemical state and composition of the fresh and treated
catalysts were studied by X-ray
photoelectron spectroscopy (XPS, SSX-100, Surface Science
Instruments, using monochromatic Al
Ka radiation). For XPS measurements, a small amount of the
scraped catalyst powder was pressed
into a piece of indium and the samples were pre-treated in high
vacuum for a few hours before
measurements. The binding energy values in the acquired spectra
were calibrated by setting carbon
1s line at 284.6 eV. Carbon and indium were excluded from the
compositional analysis. In
quantitative analysis, Shirley background subtraction was
Specific surface areas, pore sizes, and pore volumes of the
fresh and treated catalysts were
determined using the Micrometrics ASAP 2020 device. Specific
surface areas were measured from
the N2 adsorption isotherms at -196C according to the standard
method. Pore size and pore volume distributions of catalysts
were calculated from N2 desorption
isotherms by the BJH (BarrettJoynerHalenda) method.
A Fourier transform infrared (FT-IR) spectrometer (Bruker Vertex
V80) equipped with a diffuse
reflectance infrared Fourier transform (DRIFT) unit and a liquid
nitrogen-cooled mercury cadmium
telluride (MCT) detector was utilized to find the information
about the bonding of the compounds
on the scraped catalyst powder. The DRIFT analyses were
performed at room temperature under
normal atmosphere conditions. The mirror was used as a
background spectrum. Spectra were
recorded by using a resolution of 4 cm-1.
Laboratory scale light-off tests were used to define catalyst
activity before and after SW-, TA-,
TA+SW-, and SW+TA-treatments. Catalytic activities were
determined in lean reaction conditions
using the following gas mixture: 600 ppm CH4, 500 ppm CO, 10
vol-% CO2, 12 vol-% O2, 10 vol-
% H2O, and N2 as balance gas. The total gas flow was 1 dm3/min
resulting in a GHSV of 31000 h-1.
The measurements were carried out at atmospheric pressure in a
horizontally aligned tubular quartz
reactor. The temperature of the catalyst bed was increased from
room temperature up to 600C with
a linear heating rate of 10C/min. H2O was added at 110C with a
peristaltic pump. The catalyst
was kept at steady state for 15 min at 600C and after that the
furnace was cooled down to room
temperature under the N2 flow. The procedure was repeated (run 1
and run 2). If not specifically
mentioned, the data of the catalyst activities was taken from
the second run. Gas flow rates were
controlled by using mass flow controllers (Brooks 5280S). The
outlet gas composition was
analyzed as a function of temperature by a GasmetTM FT-IR gas
analyzer. Oxygen concentration
was determined by using a paramagnetic oxygen analyzer (ABB
3 RESULTS AND DISCUSSION
3.1 Structural characteristics of the catalyst
Structural characteristics of the fresh and treated catalysts
were studied by several methods. Based
on the FESEM studies, the structure of the fresh and SW-treated
catalyst was similar. Moreover, the
structures of the TA-, TA+SW-, and SW+TA-treated catalysts were
observed to be analogous.
Cross-sectional AsB images of the fresh and TA+SW-treated
catalyst are presented in Figs. 1 (a)
and (b), respectively. In the fresh and SW-treated catalysts,
the noble metal particles were too small
to be detected with FESEM. In the TA-, TA+SW-, and SW+TA-treated
catalysts, the particle size
of the noble metals was increased significantly through the
catalysts (white spots in Fig. 1 (b)).
Noble metals were still well distributed in the cross-sections
of the TA-, TA+SW-, and SW+TA-
Figure 1. Cross-sectional FESEM (AsB) images, higher
magnifications as insets, (a) the freshcatalyst and (b) the
TA+SW-treated catalyst, white spots represent the grown noble metal
Average noble metal particle sizes (diameters) of the TA-,
SW+TA-, and TA+SW-treated catalysts
were 50, 60, and 60 nm, respectively. Particle size distribution
is presented in Fig. 2. It is important
to notice that according to TEM studies, particles with the size
20 nm were taken into account in the particle size analyses
from the FESEM images because it was the minimum reliable
detection limit. Particles were
measured from the cross-sectional FESEM images with the aid of
ImageJ-software (>500 particles
with size >20 nm were measured). Thus, in the results there
is a bias towards the bigger particle
sizes. However, the results can be used in the comparison of the
large, agglomerated particles in all
TA-treated catalysts. Based on the results, sizes of the formed
large particles were similar after TA-,
TA+SW-, and SW+TA-treatments.
Figure 2. Size distribution of the noble metal particles in the
TA-, TA+SW, and SW+TA-treatedcatalysts (only particles with the
diameter >20 nm were taken into account).
Detailed structural characterization of the fresh and SW-, TA-,
TA+SW-, and SW+TA-treated
catalysts was carried out by TEMs, XRD, and XPS. In the fresh
catalyst, noble metal particles,
typically with a diameter of
Figure 3. TEM images of the fresh catalyst, (a) the
cross-sectional sample, the inset with highermagnification and
(b)-(d) the powdered sample with different magnifications.
Figure 4. STEM ADF images of the (a) fresh catalyst, (b)
SW-treated catalyst, and (c) TA+SW-treated catalyst. Notice the
different scale bar in (a) and (b) versus (c).
Figure 5. XRD patterns of the fresh, sulfur-poisoned (SW),
thermal-aged (TA), thermal-aged +sulfur-poisoned (TA+SW),
thermal-aged + sulfur-poisoned after activity
measurement(TA+SW+act.), and sulfur-poisoned + thermal-aged (SW+TA)
catalysts (g = g-alumina, d = d-alumina, q = q-alumina, and a =
Table 2. Crystallite sizes of PdO and PtPd in the fresh, SW-,
TA-, TA+SW-, and SW+TA-treatedcatalysts determined from the XRD
Size [nm] Fresh SW TA TA+SW TA+SW+act SW+TAPdO(a)
lattice parameters:a=b=3.0, c=5.3
3 6 9 914
a=b=c=3.9 - - 26 31
(a)determined from PdO-peak at 2q=33.9 with the Scherrer
equation (shape factor 0.9)(b) determined from Pd/Pt-peak at
2q=40.1 with the Scherrer equation (shape factor 0.9)
Figure 6. XPS spectra and binding energies, (a) Pd 3d, (b) Pt
4d, and (c) O 1s spectra for the fresh,SW-, TA-, TA+SW, SW-TA-
treated catalysts and TA+SW-treated catalyst after
In the SW-treated catalyst, the size of the noble metal
particles seemed to be slightly increased
(Figs. 4 (b) and 7) compared to the fresh catalyst. A slight
increase in the crystallite size of PdO was
observed also by XRD (Table 2); the amount of platinum was too
small to be detected with XRD.
According to our tentative study, no changes in the PtPd
particles of the PtPd/g-Al2O3 catalyst were
observed after 400C for 5 hours treatment in synthetic air (same
temperature and exposure time
than in the SW-treatment). Thus, a slight growth of the Pt/Pd
particles seemed to be induced by
presence of SO2 + H2O. According to the literature, sulfur and
water vapor increase the mobility of
the noble metal atoms, e.g. [18,23,24]. Based on the HRTEM
studies, mainly PdO and PtO existed
in the noble metal particles which agrees with XPS results (Fig.
6); despite the change in the
binding energy of O 1s line, it can still be attributed to
alumina . TEM-EDS point analyses
indicated both Pd and Pt in the noble metal particles as in the
fresh catalyst. The specific surface
area of the SW-treated catalyst was slightly decreased compared
to the fresh catalyst (Table 3). This
may be caused due to slight growth of the noble metal
crystallites and sulfur species blocking some
pore openings in the catalyst.
Figure 7. TEM images of the SW-treated catalyst (the powdered
sample), (a), (b), and (c) differentmagnifications.
Table 3. Specific surface area, average pore size, and total
pore volume of the fresh, SW-, TA-,TA+SW-, and SW+TA-treated
Fresh SW TA TA+SW SW+TASpecific surface area [m2/g] 154 147 96
Average pore size [nm] 10 10 14 14 15Total pore volume [cm3/g]
0.4 0.4 0.3 0.3 0.4
Significant morphological changes, due to the TA-treatments,
were detected in them compared to
the fresh and SW-treated catalysts. According to the TEM
studies, morphology of the TA-,
TA+SW-, and SW+TA-treated catalysts was similar. Based on the
XRD results, in all thermally-
treated catalysts g-alumina changed to d- and/or q-alumina and
to a-alumina (Fig. 5). Due to the
phase transformation of alumina, the particle size of
d/q-alumina and especially a-alumina
increased compared to g-alumina in the fresh catalyst. In
addition, the size of the noble metal
particles grew significantly under the thermal aging treatment
(Figs. 4 (c) and 8) as already
observed with FESEM indicating noble metal particles with a
diameter of 50-60 nm. According to
the HRTEM images (Fig. 8 (c)), the grown noble metal particles
consisted of several crystals. The
particle had a bimetallic PtPd-alloy core surrounded by several
PdO crystals. Based on the TEM-
EDS results, cores consist of both Pt and Pd and the shells are
Pd-rich. After the TA-, TA+SW- and
SW+TA-treatments, both PdO and bimetallic Pt/Pd alloy were
detected by XRD (Fig. 5). In the
TA-, TA+SW-, and SW+TA-treated catalysts, the crystallite size
of PdO was ~10 nm and that of
PtPd was ~30 nm (Table 2) which agrees very well with TEM
results. Pd was observed as an oxide
, but metallic Pt and Pd are invisible in the XPS spectra
(Figs. 6 (a) and (b)) due to the PdO
shell and the surface sensitivity of the technique. Similar
grown noble metal particles were detected
also in our earlier study concerning the lean-burn
(160000 km) . Persson et al. reported that in thermal
decomposition of PdO, Pd is incorporated
into the Pt/Pd alloy in the Pd-Pt/Al2O3 catalyst . Carrillo
et al. reported that in the thermal aging
in air at even 650C, small Pt particles formed mobile species
which migrated and were trapped by
PdO particles resulting in formation of PtPd particles .
Generally, decomposition of PtO to Pt
happens above 350C and PdO to Pd at ~800C [3,32]. Johns et al.
reported that after thermal aging
in air at 750C for 10 hours, Pt was fully reduced but almost 30
% of the Pd species were still in the
oxide form . In the thermally aged catalysts, in addition to
the grown noble metal particles there
were still also few, small noble metal particles with a diameter
of ~5 nm (Figs. 4 (c) and 8 (d)).
According to the TEM-EDS analyses, they contain both Pd and Pt
and based on HRTEM images
(Fig. 8 (d)), they seemed to be single crystals in the metallic
form indicating likely bimetallic PtPd
particles. Small, likely bimetallic PtPd particles were hard to
detect by XPS (Fig. 6 (a) and (b))
because only few these kind of particles were observed by TEM.
According to the literature ,
the position of the noble metal particles affects their
sintering so that a valley position is much more
stable than an on-top position. As a result, some particles at
the valley position do not grow even at
elevated temperature. Therefore, few small particles still
existed after thermal treatment at 1000C;
however, particles seemed to be reduced and formed bimetallic
PtPd crystallites. The specific
surface area decreased significantly (~ 40 %) and the average
pore size increased (~40 %) during
the TA-, TA+SW, and SW+TA-treatments compared to the fresh
catalyst (Table 3) due to the
significant growing of the noble metal particles and phase
transformations of the washcoat followed
by the crystal growth. SW-treatment after TA-treatment has no
further effect on the specific surface
area. It can be concluded that in the thermal treatment used in
this study, the oxidized Pt totally
reduces and partial decomposition of the oxidized Pd occurs
followed by formation of the grown
particles with a bimetallic PtPd core and a polycrystalline PdO
shell. In addition there are still also
few, small bimetallic PtPd particles.
Figure 8. TEM images of the TA+SW-treated catalyst, (a) the
cross-sectional sample, (b), (c), and(d) the powdered sample with
3.2 Sulfur species on the catalyst
According to the FESEM-EDS and TEM-EDS analyses, in the SW- and
sulfur existed uniformly through the whole catalyst structure
from the inlet part to the outlet part
and from the surface to the metallic monolith; the amount of
sulfur was ~3 wt-% which agrees well
with XPS measurements. In the SW+TA-treated catalyst, no sulfur
was detected. According to the
literature, the sulfation process is reversible and SOx from the
catalyst surface easily desorbs and
decomposes at elevated temperatures . Based on the XPS S 2p
spectrum (Fig. 9), sulfur is as
sulfates . In the O 1s spectra, the contribution of SO4
species cannot be seen due to the
domination of alumina and the possible overlapping of the
binding energies of these two . The
DRIFT spectra of the SW- and TA+SW-treated catalysts (Fig. 10)
have a broad band at around
1200-1100 cm-1 indicating bulk aluminum sulfate species [34,35].
The band around 1435 cm-1
attributed to S=O of stable Pd- or Pt-SO4 species [34,36] is
missing. Furthermore, any Pd 3d5/2
lines above 338 eV, which could be attributed to PdSO4 ,
were not detected either by XPS.
Bands around 1390-1300cm-1 attributed to surface sulfate species
on Al2O3 [16,34] or surface
Al2(SO3)3  were not observed in the DRIFT spectra. According
to Mowery et al. , sulfation
of the PdO/Al2O3 catalyst happens by oxidation of SO2 to SO3 on
PdO and SO3 can form PdSO4 on
PdO or can migrate to Al2O3 forming Al2(SO4)3. The strong band
around 1030-1040 cm-1 is due to
the catalyst material as it is present in all spectra including
the fresh catalyst. It can be concluded
that in the sulfur treatment used in this study only a small
amount of bulk aluminum sulfate formed
but no sulfur compounds on noble metals can be detected.
Figure 9. XPS S 2p spectra for the SW-, TA-, TA+SW, SW-TA-
treated catalysts and TA+SW-treated catalyst after activity
Figure 10. DRIFT spectra for the (1) fresh, (2) TA-, (3) SW-,
(4) TA+SW-, and (5) SW+TA-treatedcatalysts.
According to the EELS maps, in the SW-treated catalyst sulfur
existed mainly close to the noble
metal particles (Fig. 11 (a)) while in the TA+SW-treated
catalyst it existed randomly distributed in
the catalyst (Fig. 11 (b)). Probably, small noble metal
particles are very active to adsorb and oxidize
sulfur species and Al2(SO4)3 forms near the noble metal
particles. While, the grown noble metal
particles may be not so active to adsorb and oxidize sulfur
species resulting in that Al2(SO4)3 forms
randomly over the noble metal particles and support. According
to Smirnov et al. , at
temperatures above 300C sulfate species form on the Al2O3 thin
film without noble metal particles.
Thus, it can be assumed that Al2(SO4)3 can form also straight
with the alumina support. In addition,
due to the thermal aging treatments g-alumina changed to d-,q-,
and a-alumina which may affect
the sulfation phenomenon of the support in the TA+SW-treated
Figure 11. The STEM ADF image, the enlarged STEM ADF image, and
the STEM EELS sulfurmap from the selected area (brighter color
indicates higher amount) for (a) the SW-treated catalystand (b) the
TA+SW-treated catalyst. Notice the different scale bar in (a) and
3.3 Activity of the catalyst
Conversions of CH4 as a function of temperature over the fresh
catalyst and SW-, TA-, TA+SW-
and SW+TA-treated catalysts are presented in Fig. 12 and the
light-off temperatures (T50 and T90)
are collected into Table 4. In general, laboratory-scale thermal
treatment and/or sulfur exposure
decreased the activity of the catalyst. Methane oxidation over
the treated samples started at least
100C higher temperatures compared to the fresh catalyst and the
light-off temperatures (T50) were
observed to increase at least by 50C compared to the fresh
catalyst. The activities of the TA-, SW-,
and SW+TA-treated catalysts were similar and the activity of the
TA+SW-treated catalyst was
notably lower than that of the other catalysts. The reason why
in all the TA-treated catalyst the
activity is decreased is due to the significant morphological
changes compared to the fresh catalyst.
Due to the growing of the noble metal particles, the amount of
active sites decreased. In addition,
phase transformation of g-alumina to d/q- and a-alumina
significantly decreased specific surface
area of the TA-treated catalyst (Table 3). According to the
literature , phase transformation of g-
Al2O3 to q-Al2O3 causes the reconstruction of the surface
decreasing reactive sites of the support. In
the SW-treated catalyst, slight increasing in the size of the
noble metal particles and formation of
Al2(SO3)4 species close to the noble metal particles was
detected which are probably blocking
active sites followed by decreased conversion of methane.
According to the literature , presence
of SO2 creates Brnsted acid sites on the g-Al2O3 support while
the fresh Pd/Al2O3 catalyst has only
more reactive Lewis acid sites. Probably, this kind of changing
in the acidity of the g-Al2O3 support
happens also in our SW-treatment causing further decreased
activity of the SW-treated catalyst. In
the TA+SW-treated catalyst, these above mentioned changes in the
TA-treated and SW-treated
catalysts are combined resulting in dramatic decreasing in the
methane conversion. In the SW+TA-
treated catalyst, formed Al2(SO3)4 decomposed during
TA-treatment resulting in similar catalyst
activity to the TA-treated catalyst. Thus, formation of aluminum
sulfate randomly over the
TA+SW-treated catalyst has a significant effect on the catalyst
The catalyst activity tests were done twice (run 1 and run 2);
notable differences between run 1 and
run 2 were observed only with the TA+SW-treated catalyst. Its
activity was higher in the latter run
indicating partial regeneration, i.e. decomposition of sulfate,
of the catalyst. Thus, a short time (15
minutes) at 600C is enough to remove some sulfates from the
catalyst. According to the FESEM-
EDS analyses and XPS measurements, during the activity tests the
amount of sulfur in the TA+SW-
treated catalyst decreased from ~3 wt-% to
Figure 12. CH4 conversions as a function of temperature for the
fresh, SW-, TA-, SW+TA-, andTA+SW-treated catalysts. For the
TA+SW-treated catalyst two runs are presented.
Table 4. Light-off temperatures (T50 and T90) for the fresh,
SW-, TA-, SW+TA-, and TA+SW-treatedcatalysts. For TA+SW-treated
catalyst values are presented after the first and the second
Catalyst T50 [C] T90 [C]Fresh 390 488SW 437 550TA 445 570
SW+TA 441 552TA+SW (first run) 564 -
TA+SW (second run) 498 -
Accelerated deactivation phenomena in the PtPd/g-Al2O3
natural-gas oxidation catalyst caused by
thermal aging and/or sulfur + water poisoning were studied.
Thermal aging and sulfur + water
poisoning treatments were performed separately and with varied
characterization of the catalyst was carried out after each step
to get knowledge about existing of
sulfur and influence of thermal aging before or after sulfur
poisoning. The fresh catalyst contains
oxidized Pt and Pd particles (
water treatment before or after thermal aging. In the
TA+SW-treated catalyst, a small amount of
bulk aluminum sulfate was observed randomly distributed over the
noble metal particles and
support. In general, laboratory-scale thermal aging and/or
sulfur poisoning decreased the activity of
the catalyst. CH4 conversion curves of the SW-, TA-, and
SW+TA-treated catalysts were similar;
their light-off temperatures T50 were higher compared to the
fresh catalyst. The activity of the
TA+SW-treated catalyst was the lowest, however, the activity
recovered partly after the first
activity run (heating up to 600C) indicating partial
regeneration. Thus, combined morphological
changes and sulfate on the catalyst decreased significantly the
activity of the catalyst.
The Academy of Finland is thanked for funding (Decision numbers
138798 and 139187). The
research leading to these results has received funding also from
the European Union Seventh
Framework Programme under Grant Agreement 312483 - ESTEEM2
 P. Glin, M. Primet, Appl. Catal. B Environ. 39 (2002)
 E.M. Holmgreen, M.M. Yung, U.S. Ozkan, Appl. Catal. B
Environ. 74 (2007) 7382.
 R.J. Farrauto, J.K. Lampert, M.C. Hobson, E.M. Waterman,
Appl. Catal. B Environ. 6 (1995)263270.
 A.K. Datye, J. Bravo, T.R. Nelson, P. Atanasova, M.
Lyubovsky, L. Pfefferle, Appl. Catal. AGen. 198 (2000) 179196.
 M. Lyubovsky, L. Pfefferle, Catal. Today 47 (1999) 2944.
 Y. Ozawa, Y. Tochihara, A. Watanabe, M. Nagai, S. Omi, Appl.
Catal. A Gen. 259 (2004)17.
 K. Persson, L.D. Pfefferle, W. Schwartz, A. Ersson, S.G.
Jrs, Appl. Catal. B Environ. 74(2007) 242250.
 K. Persson, K. Jansson, S. Jars, J. Catal. 245 (2007)
 N.M. Kinnunen, J.T. Hirvi, M. Suvanto, T.A. Pakkanen, J.
Mol. Catal. A Chem. 356 (2012)2028.
 A.K. Neyestanaki, F. Klingstedt, T. Salmi, D.Y. Murzin,
Fuel. 83 (2004) 395408.
 J.K. Lampert, M. Shahjahan, R.J. Farrauto, Appl. Catal. B
Environ. 14 (1997) 211-223.
 A.T. Gremminger, H.W. Pereira de Carvalho, R. Popescu,
J.-D. Grunwaldt, O. Deutschmann,Catal. Today. (2015) 111.
 G. Corro, C. Cano, J.L.G. Fierro, J. Mol. Catal. A Chem.
315 (2010) 3542.
 D.L. Mowery, R.L. McCormick, Appl. Catal. B Environ. 34
 O. Krcher, M. Widmer, M. Elsener, D. Rothe, Ind. Eng. Chem.
Res. 48 (2009) 98479857.
 M. Konsolakis, I. V. Yentekakis, G. Pekridis, N. Kaklidis,
a. C. Psarras, G.E. Marnellos,Appl. Catal. B Environ. 138-139
 R. Wischert, C. Copret, F. Delbecq, P. Sautet, Angew.
Chemie - Int. Ed. 50 (2011) 32023205.
 C.H. Bartholomew, Appl. Catal. A Gen. 212 (2001) 1760.
 T.W. Hansen, A.T. Delariva, S.R. Challa, A.K. Datye, Acc.
Chem. Res. 46 (2013) 17201730.
 P.J.F. Harris, Int. Mater. Rev. 40 (1995) 97115.
 J.A. Moulijn, A.E. Van Diepen, F. Kapteijn, Appl. Catal. A
Gen. 212 (2001) 316.
 G.S. Parkinson, Z. Novotny, G. Argentero, M. Schmid, J.
Pavelec, R. Kosak, P. Blaha, U.Diebold, Nat. Mater. 12 (2013)
 A. Martnez, M.A. Arribas, M. Derewinski, A. Burkat-Dulak,
Appl. Catal. A Gen. 379(2010) 188197.
 A.M. Azad, M.J. Duran, A.K. McCoy, M.A. Abraham, Appl.
Catal. A Gen. 332 (2007) 225236.
 H. Arai, M. Machida, Appl. Catal. A Gen. 138 (1996)
 M. Honkanen, M. Krkkinen, V. Viitanen, H. Jiang, K.
Kallinen, M. Huuhtanen, M.Vippola, J. Lahtinen, R. Keiski, T.
Lepist, Top. Catal. 56 (2013) 576585.
 M. Aronniemi, J. Sainio, J. Lahtinen, Surf. Sci. 578 (2005)
 M. Brun, A. Berthet, J.C. Bertolini, J. Electron.
Spectrosc. Relat. Phenom. 104 (1999) 5560.
 J.Z. Shyu, K. Otto, Appl. Surf. Sci. 32 (1988) 246-252.
 J.F. Moulder, W.F. Stickle, P.E. Sobol, K.D. Bomben,
Handbook of X-ray PhotoelectronSpectroscopy, Physical Electronics,
Inc., Eden Prairie, 1995.
 C. Carrillo, T.R. Johns, H. Xiong, A. DeLaRiva, S.R.
Challa, R.S. Goeke, K. Artyushkova,W. Lei, C.H. Kim, A.K. Datye, J.
Phys. Chem. Lett. 5 (2014) 2089-2093.
 K. Hauff, U. Tuttlies, G. Eigenberger, U. Nieken, Appl.
Catal. B Environ. 123-124 (2012)107116.
 T.R. Johns, J.R. Gaudet, E.J. Peterson, J.T. Miller, E.A.
Stach, C.H. Kim, M.P. Balogh, A.K.Datye, ChemCatChem 5 (2013)
 H. Abdulhamid, E. Fridell, J. Dawody, M. Skoglundh, J.
Catal. 241 (2006) 200210.
 H. Mahzoul, L. Limousy, J.F. Brilhac, P. Gilot, J. Anal.
Appl. Pyrolysis. 56 (2000) 179193.
 S. Colussi, A. Trovarelli, E. Vesselli, A. Baraldi, G.
Comelli, G. Groppi, J. Llorca, Appl.Catal. A Gen. 390 (2010)
 M.Y. Smirnov, A. V Kalinkin, A. V Pashis, A.M. Sorokin,
A.S. Noskov, K.C. Kharas, V.I.Bukhtiyarov, J. Phys. Chem. B 109
 P. Castellazzi, G. Groppi, P. Forzatti, Appl. Catal. B
Environ. 95 (2010) 303311.
 Z. Li, G.B. Hoflund, J. Nat. Gas Chem. 12 (2003)